Electronic Properties of 0-NaV O - Rutgers...
Embed Size (px)
Transcript of Electronic Properties of 0-NaV O - Rutgers...
Electronic Properties of α′-NaV2O5
A. Gozar1,2 and G. Blumberg1,∗
1 Bell Laboratories, Lucent Technologies, Murray Hill, NJ 07974, USA2 University of Illinois at Urbana-Champaign, Urbana, IL 61801, USA
(Frontiers in Magnetic Materials (Ed. A.V. Narlikar), Spinger-Verlag 2005, pp. 697-734).
1 General properties of α′−NaV2O5 and motivation for a spectroscopic study
Introduction – α′−NaV2O5 is one of the several phases in the class of NaxV2O5 systems  and untilnow it is by far the most studied of them. Since 1996 this compound (denoted in the following simply byNaV2O5 ) has received considerable attention because it was thought to be the second realization, afterCuGeO3, of a quasi-one dimensional (1D) inorganic material displaying a spin-Peierls (SP) transition.The interest was justified given the scarcity of inorganic materials having this property, which is quiteinteresting especially for the scientific community working in the field of low dimensional quantum spinsystems. However, it turned out that the physics of NaV2O5 is more complicated and intriguing than thatand the degrees of freedom involved are not only the ones describing the spins and the lattice.
What is a SP transition? We discussed in Chapter  the general properties of a Peierls distortionwhich is a transition to charge density wave state. This means that below some temperature TP thecrystal gets distorted and the electronic density acquires a periodic spatial modulation, a process duringwhich the loss in elastic energy is compensated by the gain in the kinetic energy of the electrons. A crucialrole is played by the nesting properties of the Fermi surface (i.e. the property that enables one to connectpoints of the Fermi surface by wavevector characteristic of other excitations, in this case phonons) whichmakes low dimensional systems especially susceptible to such an instability. A pure SP transition is onein which the lattice distortion is caused by the magneto-elastic coupling, the gain in energy in this casebeing related to the spin degrees of freedom . In other words, it is a lattice instability driven by themagnetic interactions. This phenomenon leads to the formation of a spin-singlet (S = 0) ground state andthe opening of a spin-gap in the magnetic excitation spectrum, i.e. a finite energy is required to excitethe system from its ground state to lowest triplet (S = 1) state. A signature of a SP state is thus anisotropic activated temperature dependence in the uniform magnetic susceptibility below the transitionat TSP . In addition, as opposed to an usual Peierls transition, the direct participation of the spins leadsto specific predictions for the dependence of TSP on external magnetic field H . This has to do withthe fact that in the spin case the filling factor of the electronic band and accordingly the magnitude of thenesting wavevectors can be varied continuously by a magnetic field. This statement should not be takenad litteram, but in the sense that the magnetic problem can be mapped onto a fermion like system byusing a transformation of the spin operators, the magnetic field playing the role of the chemical potential,see Refs. [3, 4] for more details.
So what is the difference between CuGeO3 and NaV2O5 ? In the former, the SP nature of thetransition observed around 14 K was inferred from the exponential drop in the magnetic suscep-tibility below this temperature and especially from the dependence of TSP on an applied externalfield , see Fig. 1a. As predicted by theory, it was found that the field dependence was quadratic,1 − TSP (H)/TSP (H = 0) = α · [(µBH)/(kBTSP (H = 0))]2. Moreover, the experimental proportionalityfactor α = 0.46 was also in very good agreement with the theoretical mean field value . Finally, neutronscattering experiments and detailed investigations of the field-temperature phase diagram confirmed theprevious SP interpretation .
As for NaV2O5 , many common properties with CuGeO3 were observed. In 1996 an isotropic ac-tivated behavior below Tc = 34 K was observed by Isobe and Ueda , see Fig. 1b. Soon after that
2 A. Gozar and G. Blumberg
Fig. 1. (a) Magnetic susceptibility of polycrystalline CuGeO3 as a function of temperature for several values ofexternal magnetic fields. Inset: the reduced temperature 1−TSP (H)/TSP (H = 0) as a function of the dimensionlessparameter µBH/kBTSP (H = 0); the proportionality coefficient is 0.46. Data from Ref. . (b) Temperaturedependent susceptibility in powder samples of NaV2O5 . The inset shows the derivative dχ(T )/dT as function oftemperature for 0.1 and 5 T. Data from Ref. .
there appeared the first report of X-ray and inelastic neutron scattering (INS) data in NaV2O5 . Theauthors reported the existence below Tc ≈ 35 K of superlattice peaks due to a modulation given byk = (2π/2a, 2π/2b, 2π/4c). This wavevector characterizes distortions corresponding to unit cell doublingalong the a and b axes and quadrupling along the c direction. In the same paper, INS results showed thatthe transition is accompanied by the opening of a spin gap whose value was estimated to be ∆S ≈ 9.8 meV.So far these results are qualitatively similar to the ones in CuGeO3 but it is worth noting that a value2∆S/kBTc of approximately 6.5 already suggests a departure from the mean field value 3.52. The inter-pretation in terms of a simple SP transition became more questionable when experiments in magneticfields were performed. Note the inset of Fig. 1 where the susceptibility derivative is shown for two valuesof the external field. Specific heat measurements in chemically well characterized crystalline samples ofNaxV2O5 with 0.95 ≤ x ≤ 1 in fields up to 16 T revealed a single λ-shaped anomaly at Tc = 33.5 K andan isotropic decrease of the anomaly with ∆Tc ∝ H2 . However, the proportionality factor, the param-eter α introduced in the previous paragraph, was found to be only 20% of the mean field value . Similarmeasurements aided by magnetic susceptibility data showed a TSP (H = 0) − TSP (H = 14T ) ≈ 0.15 K,about a factor of 7 smaller than the expected value . Heat capacity measurements also pointed outincompatibilities with a simple SP transition . The authors of this paper could not reconcile the meanfield predictions of the magnetic contribution to the heat capacity with the experimental data: the specificheat jump δC/kBTc was found to be a factor of 20 higher than 1.43, which is the mean-field value, ifthe linear contribution C = γT at high temperatures was fixed to the theoretical expectations for a 1DS = 1/2 antiferromagnetic (AF) chain.
The discussion above gives us a feeling about some of the important parameters and energy scales onehas in mind when discussing the properties of NaV2O5 . The connection made with the 1D AF S = 1/2chain will get support from the description of the crystal structure which is done in the following and willbecome more clear also in the next section where other properties of NaV2O5 in the high temperaturephase are discussed. However, we conclude from what has been said that in order to explain quantitativelythe experimental findings one has to take into account other degrees of freedom, contrary to the initialbelief that at Tc one deals solely with a magnetically driven phase transition. It has become clear that thecoupling of the lattice to the charge degrees of freedom is crucial for understanding the details of what
Electronic Properties of α′-NaV2O5 3
Fig. 2. The 3D crystal structure of NaV2O5 (adapted from Ref. ). Na atoms form 1D chains along the b-axisand pairs of corner sharing VO5 pyramids pointing in the same direction form V2O5 ladder rungs. The legs ofthese ladders run along the b-axis, see also Fig. 3.
happens at Tc. The slow advance in this field was also due to the difficulty in the interpretation of X-raydiffraction data and because of a wrong identification of the crystal structure in an early study  whichgenerated a plethora of subsequent papers which were at odds with each other. Diffraction anomalousfine structure spectroscopy (also called resonant X-ray diffraction, an example of which was discussed inChapter  in connection to the existence of a density wave order in doped two-leg ladder structures)finally brought more understanding of the nature of the charge ordering in NaV2O5 , see Ref.  andcitations therein. However, in spite of years of intensive investigation of both the high and low temperaturephases of NaV2O5 , no microscopic model has successfully explained all the features of the transition and,as we will discuss in more detail, the nature of prominent excitations seen in spectroscopic experimentsas well as the light coupling mechanisms to the collective spin and/or charge excitations is still far frombeing clear.
Structure and electronic properties – The crystal structure of NaV2O5 is shown in Fig. 2. Itcontains Vanadium-Oxygen planes stacked along the c-axis and separated by Na chains. Each V-O planeis formed from pairs of edge sharing VO5 pyramids running along the b-axis (the vertices of the pyramidsin every such pair of chains are pointing in opposite direction along the c-axis), each pair being connectedin turn to a neighboring one by corner sharing pyramids. In the (ab) plane, see also Fig. 3, one canidentify two-leg ladder (2LL) units, very similar to the ones found in Sr14−xCaxCu24O41 compounds. Onecan look for instance at a pair of adjacent rows of VO5 pyramids pointing in the same direction alongthe c-axis. The rungs of the ladder, oriented along the a-axis are formed by a pair two V ions bridged byan O atom which is at the common corner of two pyramids.
Can this structure be mapped onto an array of quasi-1D electronic units? A valence counting forNa+V4.5+
2 O2−5 shows that the formal V valence is 4.5+. The electronic configuration of a neutral V atom
is 3d34s2, so a V5+ ion has a closed shell configuration while the V4+ has one 3d electron on the uppershell. On the average there is one electron shared by two V ions and this makes the 2LL’s to be at quarterfilling factor. The initially proposed non-centrosymmetric P21mn crystal symmetry group at 300 K allowed for two inequivalent V positions, interpreted as magnetic V4+ and non-magnetic V5+ sites. Themagnetic properties were thought to be determined by rows of S = 1/2 V4+ ions along a leg of a ladder(with the other one remaining magnetically inert), each row of V4+ ions being only weakly coupled toto the adjacent one due to large separation between them. It is now accepted based on X-ray diffractionstudies that above Tc the correct space group is the centrosymmetric Pmmn group [14, 15, 16]. This isimportant in what regards the number of distinct of V atoms existent in the high temperature phase:
4 A. Gozar and G. Blumberg
< = >
Fig. 3. (a) Schematic representation of the NaV2O5 in the (010) (upper figure) and (001) (lower figure) planes(from Ref. ). (b) Cartoon with the spin structure in the high temperature phase. The structure can be mappedon a weakly interacting array of quasi 1D S = 1/2 spin chains. J1 is the superexchange between neighboring spinsalong the b-axis and t⊥, t‖ and txy are the rung, leg and inter-ladder hopping parameters.
the inversion center and the the two vertical mirror planes (i. e. perpendicular to the (ab) plane) implythat there is only one type of V atoms with an effective valence of 4.5+. The fact that NaV2O5 is in amixed-valence state is further supported by nuclear magnetic resonance (NMR) studies which confirmedthe average oxidation state of all vanadium atoms to be V4.5+ .
Accordingly, one can think about the ladder structure of NaV2O5 as having on each rung an electronequally shared by pairs of V atoms forming the rungs. Susceptibility data also indicate that the couplingbetween the spins of these electrons is antiferromagnetic (AF) . The local symmetry splits the five-folddegeneracy of the d shell and makes the dxy band (the zero’s of the wave function are along the a and baxes) the lowest in energy compared to the bands generated by the other orbitals . Consequently, thedxy orbital is the relevant atomic state for the analysis of the low energy charge excitations. How aboutthe quasi one dimensionality? A density functional calculation  of the energy bands and their mappingon tight-binding models yields for the hopping terms the following values: a rung hopping t⊥ ≈ 0.38 eV,a leg hopping t‖ ≈ 0.17 eV and a inter-ladder hopping txy ≈ 0.012 eV. A difference of more than anorder of magnitude between the intra-ladder and inter-ladder wavefunction overlap is theoretical prooffor the quasi-1D nature of the system. As we will show later in relation to the low temperature phase,the dispersions of the low energy collective excitations along the a-axis, which were found to be muchsmaller than the ones along the leg direction, confirm experimentally this hypothesis. This is also trueat 300 K, as can be inferred from the band dispersions derived from an angle resolved photoemission(ARPES) study .
In a regular Fermi liquid system, the V valence would make this compound metallic. However, aninsulating character inferred from resistivity measurements was confirmed to exist both above and belowTc . This behavior is due to correlation effects  and it is explained below within a simple model.Consider a rung having one electron in a bonding orbital. The next excitation would be a transition tothe antibonding state situated somewhere about 2t⊥ above. Assuming that the on-site Coulomb energyU is infinite, i.e. no two electrons can be found on the same V d shell, an electron can hop only on anempty site of a neighboring rung. However, this will cost an energy of the order of 2t⊥. The quarterfilled ladder becomes thus equivalent to a half filled Hubbard chain with an “effective” on-rung repulsionUeff = 2t⊥ , explaining in principle why the vanadium ladders are insulating.
Electronic Properties of α′-NaV2O5 5
Fig. 4. Optical conductivity at 4, 40 and 300 K for electric fields E ‖ a (left) and E ‖ b (right) from Ref. .The letters A, B, C and D mark the main absorption features in the 0 - 4 eV energy range.
Experimental – In the following we will discuss properties of the high and low temperature phasesof NaV2O5 , concentrating on the results of our Raman scattering experiments. The single crystal wemeasured had the a × b × c dimensions around 2 × 4 × 0.5 mm and was grown as described in .Data were taken in a backscattering geometry using linearly and circularly (the latter only at the lowesttemperatures in magnetic fields) light from a Kr+ laser. All the data were corrected for the spectralresponse of the spectrometer. In addition, the resonance profile at 300 K took into account the change inthe optical properties of the material as the excitation energy ωin was swept from infra-red (IR) to violet.The incident photons propagated along the c-axis and by (xy) we denote a polarization configurationwith the incoming photon polarization ein ‖ x and outgoing polarization eout ‖ y.
2 Magnetic Raman continuum in the high temperature phase (T ≥ 34 K)
2.1 Experimental properties: polarization, resonance and temperature dependence
Before illustrating the experimental properties of the observed broad Raman continua, we show the mainfeatures of the absorption spectrum in an energy range up to about 4 eV . The absorption propertieswill be discussed in some detail because we will use these results in the analysis of our resonance Ramanstudy. Optical conductivity data from Ref.  are shown in Fig. 4. The spectra show the relevantenergy scales involving electron dynamics along and across the legs. The left panel the electric field iswas polarized along the rung direction while in the right panel the polarization was parallel to the legsdirection. The a-axis polarized spectra show a strong peak at 0.9 eV (peak A) with a shoulder at 1.4 eVand another peak at 3.3 eV (peak B). A similar, but blueshifted sequence, is observed for light polarizationalong the b direction, the energies of the observed excitations being around 1.2 (peak C), 1.9 and 3.9 eV(peak D). It should be noted that the relevant electronic orbitals to be taken into account when discussingexcitations in this energy range are the Vanadium 3d and Oxygen 2p states.
In Ref.  the authors assign peak A to an optical transition from a bonding to an anti-bondingorbital made out of symmetric (and antisymmetric) combinations of dxy orbitals of the two V atomsforming a rung. This is the fundamental gap of the optical spectrum. This interpretation was supportedon one hand by an ARPES study  which shows that the top of the bands generated by the O 2porbitals are about 3 eV below the V 3d manifold as well as by a band structure calculation  and onthe other hand, by a study of the evolution of this excitation with Ca doping in Na1−xCaxV2O5 . Ithas been observed that the spectral weight of this peak decreases linearly with Ca concentration whichis consistent with a diminishing intensity due to the fact that with two electrons per rung (Ca has a 2+valence) the many-body 2-particle state no longer allows a low energy bonding-antibonding transition. The above mentioned Ca dependence was also used to rule out the scenario that the 0.9 eV peak is aresult of V 3d ↔ 3d transition, the argument being that such an excitation would be proportional to the
6 A. Gozar and G. Blumberg
0 500 1000 1500
Raman shift (cm-1)
T = 300 K
ωin = 1.65 eV
Fig. 5. T =300 K Raman spectra of NaV2O5 in (aa), (bb) and (ab) polarizations taken using ωin = 1.65 eV laserexcitation energy.
number of V4+ ions which increases with Ca doping. If peak A is essentially an on-rung excitation, peakC at 1.1 eV was assigned to an optical excitation involving neighboring rungs . The final wave functionis different than the one corresponding to peak A because it involves combination of states having onerung with zero electrons and another one being doubly occupied, the red-shift of about 0.3-0.5 eV seenin a-axis polarization reflecting thus excitonic effects for the on-rung electron hole pair.
As for peaks B and D, they are thought to arise likely from transitions between O 2p and V 3dxy
manifolds. Remarkable is also the substantial absorption all the way up to 4 eV and even beyond whichexplains the black color of the NaV2O5 crystals. We will discuss in the following polarization, resonance ofthe Raman continuum we observe in the 0 - 200 meV energy range as well as its temperature dependence.A discussion of our proposed scenario for its origin will be contrasted to other present interpretations.
Polarization properties – Fig. 5 shows three room temperature Raman spectra taken in (aa), (bb)and (ab) polarizations and using the ωin = 1.65 eV excitation energy. The (ab) polarized spectrum hasthe lowest intensity and it is rather featureless. Next in terms of the overall background intensity comesthe spectrum in (bb) polarization. Several relatively sharp features are seen at 420, 530 and 968 cm−1 andalso some weaker ones at lower energies, 177, 230 and 300 cm−1. Besides these modes, there is a broadexcitation peaked at 680 cm−1, but not particularly strong. The sharp modes are phonons, excitationswhich were studied intensively both by Raman and IR spectroscopy . The strong continuum whichextends all the way from the origin and having a main a peak around 680 cm−1 becomes the mostprominent feature of the Raman spectrum in (aa) polarization. There are differences in phonons, forinstance in this geometry we see two modes close to 420 cm−1 as opposed to only one in (bb) configurationand also the 968 cm−1 peak is not present. We also note the observation of a smaller shoulder at about200 cm−1 and, interestingly, of another excitation around 1320 cm−1, which is approximately twice theenergy of the main peak at 680 cm−1.
Raman resonant profile at T = 300 K – In Fig. 6 we show the dependence of the intensity of thiscontinuum as a function of the energy of the incoming photons ωin. The resonance behavior is shown forthe three polarizations shown in Fig. 5. Line colors for each of the spectra shown are chosen so that theyroughy correspond to the actual color of the laser excitation beam in the visible spectrum. Besides theusual spectrometer/detector correction, the spectra shown in this figure were corrected for the opticalproperties of the crystal. The absorption coefficients the refraction indexes as well as the transmissionat the sample interface were calculated using the real and the imaginary parts of the complex dielectricfunction provided to us by the authors of Ref. . The spectral weight of the Raman continuum in the(aa) polarized spectra seems to be peaked at the extremities of the excitation range of the Kr+ laser,1.55 and 3.05 eV respectively. As for the ωin = 1.65 eV spectrum shown in Fig. 5, the broad Raman
Electronic Properties of α′-NaV2O5 7
0 400 800 12000
Raman shift (cm-1)
0 400 800 12000
0 300 600 900 12000
Raman shift (cm-1)
x 1 / 5
x 1 / 2
x 2 / 3
5 T = 300 K
Fig. 6. Raman response at T = 300 K in (aa) (left panel), (bb) (middle panel) and (ab) (right panel) polarizationsfor different incoming photon energies. Note the relative intensity scales for the three polarizations as well as themultiplication factors used for the 3.05 eV spectrum in (aa) polarization and 3.05, 2.60 and 2.34 eV spectra in(ab) configuration.
band is present also in (bb) polarization and the resonant enhancement in this configuration followsroughly the behavior in (aa) geometry. Obvious signatures of the (bb) polarized continuum can be seenfor instance in the ωin = 1.55, 1.65, 1.92 or 3.05 eV spectra, while for excitation energies correspondingto the yellow, green and blue in the visible spectrum this Raman band is absent. It is important to notethat although in cross polarization we do not observe a similar structure of the continuum as in (aa) and(bb) geometries, i.e. a broad Raman band peaked around 680 cm−1, the overall intensity of the Ramanbackground is excitation dependent, and a simple inspection of the right panel in Fig. 6 suggests thatin (ab) configuration we see a slight decrease of the background as ωin is decrease from 1.55 to 1.92 eVfollowed by an uprise at the other end of the spectrum, see the multiplication factors used for the 2.34,2.60 and 3.05 eV.
The large width of the observed continuum makes it a distinct feature compared with the othersharp phononic lines seen in the spectra of Fig. 6 and points strongly to its electronic origin. Since thephonons are not the focus of the present study, we make only a few remarks about these features at roomtemperature. The interested reader can consult Raman and IR studies in Refs. [23, 24, 25] for a detailedanalysis of their behavior as a function of polarization, excitation energy and temperature along withsome lattice dynamical calculations. In all three polarizations we observe an enhancement in the Ramanintensity of the low energy phonons in the 100 - 400 cm−1 energy range. Some of the phonons situated inthe region where the electronic Raman band is more intense have a pronounced asymmetric (Fano) shapedue to the interaction with the underlying continuum. The 531 cm−1 mode (assigned to V-Oleg stretching
8 A. Gozar and G. Blumberg
1 1.5 2 2.5 3 3.5 4
σσ σσa (10
2 ΩΩ ΩΩ−1−1 −1−1 cm
1 1.5 2 2.5 3 3.5 40
σσ σσb (10
2 ΩΩ ΩΩ−1−1 −1−1 cm
1.5 2 2.5 3
Fig. 7. (a) Intensity of the electronic Raman band (extracted from the 680 cm−1 peak hight) in (aa) polarizationas function of the excitation energy ωin (green solid circles). Dashed lines are guides for the eye. The a-axis opticalconductivity σa is plotted on the right scale (solid red line). (b) The b-axis optical conductivity σb is shown by asolid red line, and the resonant profile in (bb) polarization is shown by blue diamonds. (c) Resonance profiles in(aa) (left scale) and (bb) (right scale) polarizations from panels (a) and (b) but this time plotted together. Thesame symbols as in (a) and (b) are used. Note the blue shift of the profile in (bb) configuration. (d) The intensityof the continuum in (ab) polarization obtained by integrating the Raman response,
χ′′(ω) dω, between 100 and1200 cm−1 with the phonons masked. The optical conductivity data is courtesy of the authors of Ref. .
mode ) is proof for the interaction between the the lattice and the electronic degrees of freedom ,see for instance the spectra corresponding to excitation energies ωin ≥ 2.34 eV in (aa) polarization.
Fig. 7a-b shows the Raman resonant excitation profile for the 680 cm−1 band plotted against theoptical conductivity data, see Fig. 4 and Ref. . The red line is the the optical conductivity σ(ω) andthe same notations as in Fig. 4 are used for the main four absorption features seen in a and b axespolarized spectra. The dots represent the intensity of the Raman band extracted from the 680 cm−1 peakheight. This way of analyzing the data was chosen in the absence of a suitable fitting function for thebackground and also because of the presence of strong phononic features interacting with the continuum.The resonant enhancement towards both ends of the visible spectrum remarked in the discussion of Fig. 6,can be clearly observed here. The efficiency of the inelastic cross section follows very closely the absorptionbands, showing that this excitation is always seen ’in resonance’. Importantly, if the resonance profilesfor (aa) and (bb) polarizations are plotted together, see the inset of Fig. 7c, one can observe that the blueshift of the b-axis polarized optical peaks with respect to the peaks in the a-axis spectra is also reflectedin the dependence of the Raman band intensity as a function of excitation frequency. Although the cleanphononic selection rules we see in the data which can be easily checked for instance by comparison of crossand parallel polarized spectra, see Figs. 15 and 16, are strong reasons to believe that the (bb) continuumis not a result of sample misalignment in conjunction with polarization “leakage” from the (aa) spectra,the agreement between the blue shift seen in both the optical spectra and the resonance profile for thetwo polarizations leaves no doubt that the feature seen in (bb) data is a true Raman signal.
The 680 cm−1 peak is absent in (ab) polarization, but we still see in this case a signal which isexcitation energy dependent. This signal is not coming from spurious effects related to crystal qualityand the complete absence of scattering in the 0-2∆ energy region in the low temperature phase, where∆ = 66 cm−1 is the T = 10 K low temperature spin gap which opens below Tc = 34 K, supportsthis statement. In Fig. 7d we show the integrated (ab) polarized Raman response χ′′(ω) between 100 and1200 cm−1 with the sharp phononic features masked. As was the case for the data in parallel polarizations,we observe again an enhancement in the background for the lowest and highest excitation energies ωin.
According to the interpretation of the optical features seen in Fig. 4, the intermediate electronicstates responsible for the resonant behavior involve on-rung bonding-antibonding transitions, inter-rungexcitations as well as transitions from the lower O 2p states to the V 3d bands. Irrespective of the
Electronic Properties of α′-NaV2O5 9
0 200 400 600 800 1000
Raman shift (cm-1)
T > Tc
T < Tc
Fig. 8. (a) Raman scattering continuum in NaV2O5 taken in (aa) polarization at 300, 200, 100 and 45 K usingthe ωin = 1.83 eV excitation energy. Note the softening of the band peaked at 680 cm−1 at room temperatureas well as the development of another continuum at frequencies below 200 cm−1. The sharp modes are phonons.(b) Cartoon showing the average distribution of the valence electrons provided by V atoms (represented by solidblack dots) within a given ladder above (left) and below the transition (right). The picture on the right does notshow the additional lattice dimerization and the alternation of the nearest neighbor superexchange J1, see thefollowing section for a more detailed discussion of the low temperature phase.
interpretation, we established so far that the continuum peaked at 680 cm−1 appears in both (aa) and (bb)polarizations, the peak is not present in cross polarization and is a strongly excitation energy dependentfeature, which allows us to clearly see its next overtone for incoming photon frequencies ωin ≥ 2.6 eV orωin ≤ 1.65 eV.
Temperature dependence for 34 < T < 300 K and the role of fluctuations above the
critical temperature – We show in Fig. 8a the dependence on temperature of the Raman continuumas we cool down from 300 K to just about the transition. The data are taken in (aa) polarization and theexcitation energy used was ωin = 1.83 eV. We remark two effects regarding this spectra. The first is thedownshift with cooling of the strong Raman band in the 680 cm−1 region accompanied by an increase inits spectral weight from the low energy side. Although the interaction with the 530 cm−1 phonon maylead to an additional shift compared to its “bare” energy, one can observe by simple inspection of thespectra a substantial softening of about 80 cm−1 with cooling from 300 to 45 K. No qualitative changesin the band are seen with further decreasing temperature below the transition.
The second effect is the appearance of another band below 200 cm−1. The 0-200 cm−1 energy regionis important because this is where many new collective excitations are seen below Tc = 34 K as a resultof lattice distortions and the opening of the spin gap. By now it is established that below Tc the in-planeordering of the spin/charges on the outer Vanadium d shell involves, in each ladder, a zig-zag patternlike the one shown in Fig 8b . The band at low energies can thus be understood as a precursorof the strong and sharp collective modes in the ordered phase, see Section 3. It is important that thiscontinuum exist in an incipient form at 300 K and can be clearly seen already at 200 K. Similarly withthe band peaked at 680 cm−1, this low energy counterpart gains substantial spectral weight from the lowenergy side with cooling. We consider the data in Fig. 8a as proof that the transition at 34 K is precededalmost up to 300 K by strong fluctuations of the low temperature order and suggest that the reason thecritical temperature is so low is not because of intra-ladder dynamics, but it is rather due to the phasingof the zig-zag charge order between coplanar and inter-layer ladders. This statement is supported byfrequency and temperature dependent electron spin resonance (ESR) linewidth, see Ref. . At 36 Kthe authors of this work estimate a characteristic frequency of about 700 GHz (≈ 25 cm−1), for theprecursor fluctuations.
10 A. Gozar and G. Blumberg
We also note that the topology of the ladder at quarter filling and the charge pattern below Tc
suggest that other magnetic terms are important beside the nearest neighbor exchange J1 shown inFigs. 3b and 8b. For instance, if one compares in Fig. 8b the low temperature exchange path between twoV atoms sitting on two adjacent rungs (which is related to J1) to the exchange path between next nearestneighbors (which is related J2), one can argue that the difference may not necessarily be large. On thecontrary, the superexchange J2, taking place on a straight line across one vanadium and two Oleg atoms,could be comparable to J1. A quantitative estimation of possible competing interactions would be verywelcome and important for the interpretation of the magnetic excitation spectrum. The statements aboutthe importance of other magnetic terms is supported by measurements of the temperature dependentmagnetic susceptibility and its comparison with the theoretical expectations within the model of 1D AFHeisenberg chains characterized only by nearest neighbor exchange, see Ref. . The authors of thiswork show that the measured susceptibility χ(T ) above 34 K is not in good quantitative agreement withthe predictions of S = 1/2 uniform Heisenberg chain with only nearest neighbor interaction. The data canbe reconciled with theory only if additional magnetic exchanges are included and/or the superexchangeitself is temperature dependent. In view of the discussion above, we believe that a significant temperaturedependence of the effective magnetic interactions as well as of the relative importance of competingexchange terms could be understood if one invokes the increasing charge imbalance on each V-O-V rungwith cooling.
2.2 Interpretation of the Raman continuum in terms of multi-spinon Raman scattering
In discussing the nature of the Raman band we have to acknowledge the existence of a substantialbody of prior spectroscopic (Raman and IR) work, see for instance Refs. [22, 23, 24, 25, 27], as well asconcomitant or subsequent to our study [28, 29]. Interesting properties were observed in addition to whathas been discussed in the previous section. One of them is its dependence on the Na concentration inNaxV2O5 crystals . With a decrease of the Na concentration a pronounced weakening in the continuumintensity as well as a downshift in energy from 680 to about 480 cm−1 has been observed as x was variedfrom from 1.0 to 0.85 (and implicitly decreasing the number of rung electrons). Another property isrelated to the presence of a broad continuum of excitations in the far IR part of the optical conductivitydata, extending from very low frequencies (below about 100 cm−1) almost up to the electronic excitationsseen around 1 eV, when the electric field was parallel to the a-axis . This continuum, whose energyscale resembles much the one seen in Raman spectra, was interpreted by the authors of Ref.  in termsof “charged two-magnon” excitations. In order to insure an electric dipole coupling to these double spinflip excitation the authors had to introduce a rather artificial charge asymmetry between the legs of eachladder, represented by an energy difference for the single particle on-site energy depending if it sits on theleft or right of the V-O-V rung. Moreover, the model, which includes the hopping parameters t⊥ and t‖together with Coulomb repulsion U for double site occupancy, neglects the Coulomb interaction betweennearest neighbor sites which seems to be an important ingredient for the analysis of charge dynamics ofthe quarter filled ladder . While the energy scales certainly suggest a common origin for the Ramanand IR continua, the interpretation of both of these features is a matter of debate.
The common interpretation of the Raman continuum is that it is related to Raman active transitionsbetween crystal split d levels of the V atoms [25, 28], while the interaction with the phonons resulting inthe so called Fano shape is due to electron-phonon coupling. This assignment is not however based onspecific calculations. On the contrary, its energy scale seems to be too low as band structure calculations show that the splitting between vanadium d bands involves energies at least of the order of 2500 cm−1.The temperature dependence showed in Fig. 8 remains also unexplained in this scenario. In fact, it waspointed out in Ref.  that with cooling the broad band should recover the discrete nature of anexcitation between well defined atomic electronic levels. The band remains however broad to the lowesttemperatures (around 5 - 10 K) measured.
Although the possibility that the Raman continuum has a magnetic origin was mentioned in literature,this idea has been ruled out, see Refs. [25, 27, 28] and the main argument was that this excitation appearsonly in (aa) polarization and it is not present in (bb) polarization. The latter geometry was considered theexpected scattering configuration where a two-magnon type excitation should be observed if one takes
Electronic Properties of α′-NaV2O5 11
into account the spin structure shown in Fig. 3b and also the fact that, according to the Fleury-LoudonHamiltonian [30, 31], the b-axis is parallel to the dominant exchange path. A second reason was that a two-magnon continuum peaked at 680 cm−1 would yield a value of the nearest neighbor superexchange J1 toolarge in comparison to estimations from magnetic susceptibility  and inelastic neutron scattering .We will return to this issue later in this section. For the moment we mention that it was demonstrated inFigs. 6 and 7 that the continuum, although weaker, is present also in the configuration when the incomingand outgoing photons are parallel to the ladder legs. Moreover, a strong argument in our view against d tod transitions is the presence of the second overtone of this excitation around 1320 cm-1, see Fig. 5, whoseweaker intensity suggests that it results from second order scattering. There is no intrinsic reason thatthe crystal field split bands are distributed in such a way that another set of Raman allowed transitionsis to be found at exactly double the frequency of the main peak. Finally, there is a counterpart of thisRaman continuum in the spin-Peierls compound CuGeO3 whose origin is generally agreed on to be indouble spin-flip processes . The different energy scales of the continua in CuGeO3 and NaV2O5 canbe understood in a simple way if one takes into account the ratio of the dominant magnetic exchangeinteractions in these two compounds.
The above arguments allow us to propose that the origin of the Raman band peaked at 680 cm−1 ismagnetic and that it represents a two-magnon like continuum of excitations. Moreover, we will show in thefollowing that this assignment is compatible with its temperature dependence, resonance and polarizationproperties, which further strengthen the identification of the origin of this band as magnetic. We will alsodiscuss the possibility of reconciling the obtained value for the magnetic superexchange with the onesexistent in the literature. Given the fact that in the high temperature phase NaV2O5 can be mapped ontoan array of weakly interacting S = 1/2 AF chains (see Fig. 3), we will discuss first their characteristicexcitations within the Heisenberg model.
Excitations out of a quasi 1D S = 1/2 AF chain and the two spin-flip Raman continuum –
The purpose in this part is to show that a broad band as observed experimentally is consistent with thetheoretical predictions for spin-flip excitations in a 1D AF S = 1/2 chain. Consider a system like inFig. 8b and the Hamiltonian:
H = J1
Si · Sj + J2
Si · Sj (1)
where Si and Sj represent spins on chain sites i and j respectively while NN and NNN stand for nearestneighbor (j = i ± 1) and next nearest neighbors in the same ladder (j = i ± 2). J1 and J2 = αJ1 are thecorresponding superexchange integrals and we consider the case where both of them are positive. TheNNN term leads to spin frustration, but due to the larger spatial separation in the high temperaturephase it is generally expected that J2 is only a fraction of J1. Let us look at the J2 = 0 case first. Theexcitations out of a S = 1/2 1D AF chain in this limit are gapless domain wall solitons called spinonswhich have a dispersion given by ω(k) = πJ
2 | sin(k)| . Spinons carry a spin of 1/2 and they can becreated only in pairs, each pair corresponding to one spin flip and thus having integer spin. In some senseone can think about a magnon like excitation as being composed out of two spinons. Similarly, a statewith two spin flips (two-magnon Raman scattering) would correspond to the creation of four spinons.Figure 9a shows the excitation spectrum of the spinons and the continuum of two-particle excitations.Panel b is an intuitive visualization of a two-spinon excitation carrying a total spin S = 1.
Here we come back again to a remark made in Chapter : which way provides a better descriptionof the spin dynamics, one that starts from true elementary excitations (in our case the spinons whichare fractional spin excitations) or a description in terms of elementary triplet (S = 1) excitations, whichare bosonic modes (corresponding to the known textbook magnons in the case where there is long rangemagnetic order and a semi classical approach applies)? This question is probably most relevant for theS = 1/2 1D AF chain with only NN interactions because this is the archetype of a gapless critical modelwhose true elementary excitations are known to be the spinons, and not triplons (elementary triplets). This question was addressed by the authors of Ref. , who perturbatively calculated spectraldensities for various operators R connecting the ground state to states with different number of excitedtriplets according to: I(ω) =
f | < f |R|0 > |2δ(ωf − ω0 − ω) = −π−1Im[< 0|R(ω + ω0 − H)−1R|0 >]where H is given by Eq. 1 with J2 = 0, |f > and |0 > denote excited and the ground state while ωf
12 A. Gozar and G. Blumberg
Fig. 9. (a) Excitation spectrum of a 1D S = 1/2 AF linear chain with nearest neighbor Heisenberg exchangeJ . The lower line, (πJ/2)| sin(k)| is the dispersion for one spinon. The πJ | sin(k/2)| curve marks the higherenergy edge of the two-spinon continuum. (b) Cartoon with a two spinon excitation. 1 and 2 are two degenerateconfigurations in the AF ground state. The two spinon excitation in the lower part can be thought of as a pair ofdomain walls between regions of type 1 and 2. The total spin of this state compared to the states 1 and 2 amountsto one spin flip.
and ω0 represent their energies. Using a continuous unitary transformation which conserves the numberof elementary triplets and appropriate interactions R, they could evaluate separate relative contributionsto Itot =
0dω I(ω) =
∑∞n=1 In from sectors with only one, two and three triplets (the total intensity
being calculated using the sum rule Itot =< 0|R2|0 > − < 0|R|0 >2). The main result was that thesum rule is very well fulfilled by taking into account only the contributions up to (and including) threetriplets , implying that there is no necessity to resort to fractional excitations. It would be interestingto check if this statement remains true at all energies, an issue which could be addressed probably byevaluating relative contributions to energy and wavevector dependent spectral densities, I(k, ω).
How does the excitation spectrum evolve with increasing the NNN frustrating parameter α = J2/J1?It turns out that for 0 ≤ α ≤ αc the excitation spectrum remains gapless and qualitatively the same as inFig. 9  and the true excitations are again spinons. However, there is a critical value αc ≈ 0.24 abovewhich the low energy spectrum develops a finite spin gap. The spin-spin correlations become short rangedfrom the power law fall-off characteristic of the uniform unfrustrated chain. For an intuitive picture, thevalue α = 0.5 is very interesting because in this case the ground state is doubly degenerate and it isknown exactly to be made of products of NN singlets. In the notation of Eq. 1, this means that for thisvalue of α the two degenerate ground states are |0 >1= 2N/2
∏Ni=1(| ↑2i−1> | ↓2i> −| ↓2i−1> | ↑2i>)
and |0 >2= 2N/2∏N−1
i=1 (| ↑2i> | ↓2i+1> −| ↓2i> | ↑2i+1>). The value of α = 1/2 for 1D chains is knownas the Majumdar-Ghosh point . This is also the moment to advertise the compound discussed inChapter , SrCu2(BO3)2, which is the only experimental realization of a two-dimensional structure,well described by a NN and NNN Heisenberg terms, having an exactly known ground state. Similarlyto the 1D case, this ground state can be also written in terms of independent nearest neighbor singletstates.
As it is also discussed in the Chapter , in the absence of spin-orbit coupling and because of thespin selection rules, Raman scattering usually couples to double spin flip states via the photon inducedspin exchange process [30, 31]. The effective spin Hamiltonian corresponding to this interaction in theoff-resonance regime is given by:
(ein · rij)(eout · rij)Si · Sj (2)
where rij is the vector connecting these sites and ein/eout are the unit vectors corresponding to theincoming/outgoing polarizations. Because the light wavevector is very small, the total momentum of theexcitations probed has to be zero. From Fig. 9 one can infer that the energy range spanned by four spinon
Electronic Properties of α′-NaV2O5 13
Fig. 10. (a) Raman intensity for four spinons evaluated with different matrix elements, M =cos(Q/2), 1, cos(Q), cos(2Q), from Ref. . A nearest neighbor (NN) Fleury-Loudon interaction (Eq. 2) cor-responds to M = cos(Q) and a next nearest neighbor (NNN) interaction to M = cos(2Q). (b) Raman intensityfor the Heisenberg model (Eq. 1) for various ratios of the NNN exchange J2 with respect to the NN term J1. Notethat an increase of J2/J1 results in a downshift of the four spinon continuum spectral weight. The results in thispanel are also from Ref. .
excitations with zero total momentum is quite large: from ω = 0 up to ω = 2πJ . One also expects thatthe Raman form factor is peaked in the middle of this region, at ω = πJ , reflecting the divergence inthe spinon density of states at this energy. The large energy range corresponding to the multi-spinoncontinuum along with the well established inelastic light coupling to double spin flip excitations is thuscompatible with the existence of the broad Raman continuum observed in Figs. 5, 6 and 8.
In fact numerical calculations using the Hamiltonian Eq. 1 and an interaction of the form Hint ∝∑
i Si · Si+2 revealed that the Raman intensity corresponding to the four spinon excitations correspondsindeed to broad continuum like feature, see Fig. 10a and Ref. . Note that this interaction is nothingelse but a particular form of Eq. 2 for (bb) polarization (polarization along the chain direction) where aNNN term was chosen. It is also important to observe that because of the commutation relations withthe system Hamiltonian, the interaction Hint could have been as well chosen to be Hint =
i Si · Si+1,i.e. to describe spin exchange between NN spins, but in this case it would have been necessary to includeNNN terms in Eq. 1 so that [H, Hint] 6= 0. While the exact shape of the four-spinon continuum fromFig. 10a does not exactly correspond to the experimental findings in NaV2O5 (Figs. 5 and 6) or CuGeO3
(Ref. ), it nevertheless proves that the four spinon Raman continuum is an excitation relevant onan energy scale ranging from zero up to energies of about 6J (which corresponds to the 0 − 2πJ rangeinferred from Fig. 9). The overestimation of the low energy spectral weight has to do with the choice forthe Raman matrix elements. One can compare Fig. 10a with results obtained by exact diagonalizationand/or mean field approximation for the frustrated spin chain [40, 41]. These calculations reproducebetter the experimental findings because the divergence at πJ is replaced by a broader peak and alsobecause they eliminate the preponderant low frequency part.
Discussion of the temperature dependence – Here we intend to show that the temperaturedependence from Fig. 8a is also consistent with an interpretation of the continuum in terms of multi-spinonexcitations. The experimental observation there was related to the softening of the Raman band withcooling from room temperature to about 40 K. An interesting connection can be made between Fig. 10band the discussion about the role of fluctuations and higher order magnetic exchange terms regardingthe results in Fig. 8a-b. In this respect, note also that, according to Eqs. 1 and 2, the inclusion of termsbeyond the nearest neighbor (either in the system Hamiltonian or in the interaction Hamiltonians) arecrucial for observing any inelastic magnetic signal.
Fig. 10b shows that there is a substantial overall downshift in the four-spinon spectral weight withincreasing the NNN frustrating interaction J2. When we analyzed the data in Fig. 8a-b we broughtevidence that the fluctuations of the low temperature order start at high temperatures and also that
14 A. Gozar and G. Blumberg
magnetic susceptibility results cannot be understood if only the NN exchange J1 is taken into account. Inparticular, we discussed that the tendency of the charges to arrange themselves in a zig-zag pattern canmake the NNN exchange J2 an important parameter. So the reasoning goes as follows: (1) decreasing thetemperature leads to a more and more pronounced charge disproportionation along the left and right legsof the ladder; (2) this may lead on one hand to a decrease of J1 because the exchange path gets modified(the two electrons on a rectangular plaquette formed by two rungs will like to stay along the diagonal)and on the other hand to a relative increase of J2 because the NNN Vanadium atoms become connectedby a straight, shorter superexchange path; (3) according to Fig. 10, both effects in (2) will lead to asoftening of the four spinon Raman continuum. While still speculative (in the absence of a quantitativeestimation of the charge imbalance as a function of temperature or of quantitative microscopic calculationsof the relative strengths of the magnetic interactions) our point was to provide a possible basis for theunderstanding of the data in Fig. 8.
Discussion of polarization properties – In a strictly 1D system, because any two spin sites canbe connected only by vectors rij ‖ b-axis, the Fleury-Loudon polarization selection rules (Eq. 2) wouldnot allow coupling in a polarization perpendicular to the chain direction, the (aa) configuration. However,we do observe scattering in this geometry.
Here is the place to reiterate some issues about the symmetry of the high temperature phase. Theimportance of symmetry resides in the fact that it is the most direct way to establish the spin/chargepattern above Tc. We discussed in the introduction that more recent X-ray scattering as well as NMRdata support a centrosymmetric group in the high temperature phase and the existence of only onetype of V atoms with an average valence of +4.5. This means that, because the rung hopping t⊥ is thedominant term compared to the inter-ladder hopping txy or the overlap along the chain direction t‖ ,on each rung there is only one electron which is rapidly hopping from the left to the right side making(averaged over the timescale characteristic of each experimental probe) the two rung vanadium atomslook equivalent. At a quantum mechanical level, one can think about the electronic wavefunction as asuperposition of ’instantaneous’ states having electrons arranged in different configurations so that whenthe charge density is averaged over the left and right legs of the ladder one gets (almost) equal fractionalcharges q = e/2.
In spite of the preference of the centrosymmetric group Pmmn [9, 14, 15, 16] over the P21mn group, this assignment is not entirely unambiguous and the analysis of the X-ray data becomes quiteinvolved because both the crystallographic symmetries render almost identical diffraction patterns . Infact a small, finite charge imbalance between V-O-V ladder legs existent even at room temperature couldnot be completely excluded. This is fully consistent with the Raman data in Fig. 8 which shows thatthe effects of the fluctuations of the low temperature zig-zag order can be tracked down at all measuredtemperatures above Tc = 34 K and that this temperature has to do mostly with the inter-ladder phasecoherence. This in turn means that locally and on relatively short time scales the charge pattern on eachladder is different from the average distribution seen by X-ray diffraction and that a cartoon for the hightemperature phase like the one shown in Fig. 3 is only an idealized approximation.
If one agrees with the notion that inside each ladder the charge/spin distribution is not strictly 1D,then the selection rules derived from Eq. 2 allow scattering in (aa) polarization. So four spinon continuumshould be seen in both (aa) and (bb) geometries, consistent with our experimental observations. This alsoimplies that the temperature dependence of the magnetic Raman band should track the evolution of thezig-zag order in the V-O planes, in particular we should observe an increase of its spectral weight withcooling, a process driven by closer proximity to the low temperature phase. This is one aspect we alreadynoted when discussing the Raman results, i.e. that the softening of the 680 cm−1 peak is also accompaniedby an increase in the spectral weight on the lower energy side. Once the selection rules allow it, the peakin (aa) can be imagined as being the result of the well known phonon induced spin exchange process: anelectron-hole pair is created by an electron dipole interaction involving bonding-antiboding V 3d orbitalsand O 2p bands, see Fig. 4; in the intermediate state two pairs of spinons are emitted before the collapseinto an excited spin state. Why is the signal in (aa) stronger than in the expected geometry (bb)? This hasto do with the fact that the coupling when the electric field is perpendicular to the ladder is different fromthat along the b-axis and this is especially the case with the Raman vertex in resonance conditions. Weshowed in Fig. 6 that the intensity of the Raman band follows very closely the features seen in absorption,
Electronic Properties of α′-NaV2O5 15
so one cannot talk about off-resonant conditions. In this respect we note that quite different couplings in(aa) with respect to (bb) polarization of fully symmetric excitations are also observed for phonons, seeFig. 5. It is known from the case of 2D cuprates that very strong enhancements of the magnetic signal canoccur  and they have been observed in resonant Raman spectra . A quantitative understandingof the anisotropy in the (aa) and (bb) intensities would require specific evaluations of the Raman matrixelements, but in principle it is compatible with our observations
A zig-zag pattern also implies finite magnetic scattering in (ab) polarization. In Fig. 7d we show thatthe integrated intensity in this geometry is excitation energy dependent, but the 680 cm−1 peak is notobserved. In fact this is not surprising, because the spin flip scattering in cross polarization should havea different form factor and it belongs to a different irreducible representation in an orthorhombic group.As a result, it is a priori expected to have a different spectral shape than in parallel polarization. Dueto the distinct form factor in different scattering configurations, the Raman intensity integrates fromdifferent parts off the Brillouin zone and symmetry properties may lead to the cancellation of the zoneboundary divergence in the density of states at πJ . Examples in this regard are again the 2D cuprateswhere the inclusion of terms beyond the nearest neighbors in the effective light coupling Hamiltonianled automatically to the appearance of magnetic scattering not only in B1g, but also in A1g and B2g
symmetry channels . However, the spin pair scattering in each channel comes in with its own resonanceand spectral properties.
Evaluation of the magnetic superexchange – The peak position of the four spinon continuumat 680 cm−1 (84 meV) (see Fig. 5) and the expected maximum in the Raman response at πJ1 reflectingthe divergence in the density of states (see Fig. 10a) lead to an estimation for the NN superexchangeJ1 ≈ 27 meV (218 cm-1 or 310 K). Given the spectral weight downshift induced by the presence of theNNN term J2 (Fig. 10b) we can say that this value is a lower bound for the NN superexchange. Ourvalue is in good agreement with the initial determination of J1 from a fit to the magnetic susceptibilitydata  by the Bonner-Fisher prediction (Ref. ) as well as with the estimation from charged bi-magnon continuum observed in the optical conductivity data . The interpretation of the IR absorptiondata relies on a global charge asymmetry between the ladder rungs. Seemingly artificially introduced,this assumption may be regarded retrospectively in a more favorable light in the context of strongfluctuations of the low temperature order. It is also possible that the difficulties in a precise distinction ofthe symmetry in the high temperature phase can be related to the same phenomenon. As for the magneticsusceptibility data from Ref. , it was pointed out in a more recent paper, Ref. , that it could notbe reproduced quantitatively in subsequent studies. Moreover, the authors of this latter work obtainedfrom an approximate fit (because they argued that the data cannot be quantitatively fit by a simpleBonner-Fisher expression involving only NN Heisenberg interactions) a value for J1 which is almost twiceas high as ours.
A fit to the experimental dispersion of the elementary triplet excitation in the low temperature phaseobtained in a INS study, see Ref. , allowed the extraction of a value J1 ≈ 60 meV, also about a factorof two higher than 27 meV. Regarding this data we note that the maximum neutron energy transfer was40 meV while the inferred maximum for the triplet dispersion was 93 meV. Accordingly, the value of theenergy at the zone boundary, which is of crucial interest to us (see Fig. 9), was not determined directlybut only by using an approximate fitting function . Neither the authors of the INS work, nor those ofRef.  consider the possible influence of NNN exchange terms which we believe play an important rolein determining the structure of the magnetic excitation spectrum.
We conclude by saying that our estimation for the lower bound of the superexchange, while not con-tradicting other analyses, is still too far apart to be explained by error bars. In our view, a quantitativedetermination of the relevant J ′s is still an open issue and the underlying reason is in the stronglyfluctuating low temperature order and the induced frustration effects. We also believe that the overallconsistency between the interpretation of the strong Raman band in the high temperature phase in termsof multi-spinon excitations and our experimental findings strongly argues for its magnetic origin.
16 A. Gozar and G. Blumberg
0 200 400 600 800 1000
Raman shift (cm-1)
0 50 100 150 200
Raman shift (cm-1)
0 100 200 3000
0 - 290 cm-1
Fig. 11. The main panel shows the Raman response χ′′(ω) in (aa) polarization for T = 45 and 5 K. The datais taken using the ωin = 1.92 eV excitation energy. Left inset: Temperature dependence of the (aa) polarizedspectra in the 0-250 cm−1 region. The data for 45 and 5 K are zoomed in spectra from the main panel. Rightinset: Integrated intensity,
χ′′(ω) dω, between 0 and 290 cm−1 as a function of temperature.
3 Collective excitations in the low temperaturephase of NaV2O5 (T ≤ 34 K)
3.1 General features of the transition
In the main panel of Fig. 11 we show two Raman spectra taken at 45 and 5 K in (aa) polarization. Onecan notice that drastic changes occur across the transition at 34 K especially at low frequencies wheremany new modes appear. The most prominent three features below 150 cm−1 are a very strong mode at66 cm−1, another one around 105 cm−1 and the sharp edge at 134 cm−1 (≈ 2·66 cm−1) marking the onsetof a continuum. Other new excitations which are clearly seen in the T =5 K spectrum are found around166, 202, 308, 332, 393 and 949 cm−1. Besides these modes, other weaker excitations are seen around 122and 182 cm−1. In Fig. 8 we argued that the strong temperature dependence in the low frequency part ofthe spectra and the development of the low frequency continuum between 0 and 250 cm−1 is a precursorfeature signaling fluctuations of the low temperature order at temperatures above Tc. That this is truecan be seen in the left inset of Fig. 11 which shows that below about 34 K, this broad excitation ’splits’into very sharp resonances. While above Tc the individual ladders do not know about each other at largedistances, below 34 K a global phase coherence of the charge and lattice dynamics is established. Also,the drop in the 0-200 cm−1 continuum marks the opening of a gap in this energy region. The integratedRaman response in the 0-290 cm−1 region,
χ′′(ω) dω shown in the right inset of Fig. 11, increases withdecreasing T almost all the way down to the lowest measured temperature, their weight relating mostprobably to the variation of the charge/spin order and lattice distortion in the low temperature phase.
How are these changes to be understood and what are the energy scales below Tc? As for the crystalstructure it is known that in the V-O layers there is a doubling of the unit cell along both the a and bdirections [7, 12, 46]. Moreover, in every ladder there is a zig-zag type ordering of the Vanadium valenceelectrons rendering, crudely speaking, V4+ and V5+ atoms on each rung of the ladder, see one rectanglein Fig. 12a. Given the 2a× 2b supercell, there are exactly four realizations of this superstructure in each
Electronic Properties of α′-NaV2O5 17
J1(1 + δ)
J1(1 - δ)
J2 = α J
Fig. 12. (a) Schematic representation of the 3D charge/spin order (from Ref. ). Black (open) circles are V4+
(V5+) atoms. Each of the four rectangles shown represents a unit cell in the low temperature phase. The sequenceB D A C represents one of the stacking sequences along the c-axis which are consistent with X-ray diffractiondata, i.e. it has to the inter-layer phasing of the zig-zag order in each layer. Note the doubling (along a and bdirections) and the quadrupling of the unit cell along the c-axis. (b) Cartoon with the zig-zag order and relevantintra-ladder magnetic interactions. The parameter δ characterizes the dimerization of the superexchange due tothe unit cell doubling along the ladder legs. Inter-ladder interactions are not shown.
plane, and they are denoted by A, B, C and D. The existence of four such possibilities to accommodatethe zig-zag order provided a clue for the understanding of the quadrupling of the lattice constant alongthe c-direction. Initially an average face centered orthorhombic structure was proposed to explain theX-ray data at low temperatures . The authors proposed a stacking disorder pattern along the c-axis rendering an effective global orthorhombic structure characterized by the face centered space groupFmm2. However, this group has two mirror planes parallel to the c-axis which is at odds with the zig-zag order in each plane. The resolution of this problem suggested in Ref.  was that because X-raysare sensitive only to the average structure, a model lacking mirror symmetry in each plane but havingthe appropriate stacking disorder along the c axis can be in accordance with the measured diffractionpattern. A later resonant X-ray study argued for a lower (monoclinic) symmetry of the low temperaturestructure and proposed only two almost degenerate stacking patterns perpendicular to the ladder planes. One of them, the B D A C model is shown in Fig 12a. It was proposed that the true crystal structurebelow Tc involves the existence of stacking faults of different possible patterns. The data was suggestedto reflect the presence of competing arrangements along the c direction of nearly degenerate units. Thismay lead to a rich phase diagram as a function of a parameter which could directly affect the inter-layerinteractions. Indeed, X-ray diffraction data under pressure, see Ref. , show the development of a seriesof modulation wavevectors corresponding to an array of commensurate phases in the P − T diagram.The complicated observed sequences were qualitatively understood within the devil’s-staircase-type phasetransitions driven by two (presently unknown) competing interactions along c.
The above details and the discussion in the previous section give an idea about the difficulty in un-derstanding quantitatively what exactly happens with the structure both above and below the transition.However, what can be surely said about the changes in the in-plane magnetic interactions as a result ofthe transition? A qualitative picture of what happens inside a given ladder can be obtained from Fig. 12b.The unit cell doubling along the b direction leads to an alternation in the NN superexchange J1 whichis quantified by the parameter δ. Due to the particular arrangement of charges in the zig-zag pattern,it seems that the NNN term may also play an important role in the spin dynamics. The single ladderhamiltonian can be thus written as:
H = J1
[(1 + (−1)iδ)Si · Si+1 + αSi · Si+2] (3)
18 A. Gozar and G. Blumberg
π/b0 π/b0 π/2b
Fig. 13. (a) Cartoon showing the dispersion of the elementary excitations (spinons) in a uniform S = 1/2 AFchain (the same as in Fig. 9a). (b) Qualitative changes in the (slightly) dimerized Heisenberg chain. The unitcell along the chain becomes 2b and the alternation of superexchange is given the parameter δ (the same as inFig. 12). The elementary excitations are S = 1 triplets and a spin gap ∆ opens up at the Brillouin zone center.Apart from logarithmic corrections, ∆ scales as δ2/3 .
The charge/spin order coupled to the lattice dimerization in the direction perpendicular to the ladders maylead to a complicated 2D pattern of magnetic exchanges (see for instance the discussion in the caption ofFig. 14). However, assuming a relatively weak inter-ladder coupling, which is confirmed experimentally bythe small dispersion of the magnetic modes along a-axis, one can assume that the backbone Hamiltonianfor the magnetic interactions is given by Eq. 3, i.e. a dimerized and frustrated 1D AF S = 1/2 chain.
We will discuss later the excitations from dimerized and frustrated chains in more detail. This topichas been the focus of many theoretical studies [48, 49, 50]. Here we are preoccupied only with the mainresult of the dimerization of the NN exchange, which is shown in Fig. 13a-b. If in the uniform case,panel a, the excitation spectrum is gapless (see also Fig. 9), any finite dimerization δ will open up a spingap at the Brillouin zone center. This gap, denoted by ∆, scales as ∆ ∝ δ3/2 apart from logarithmiccorrections [48, 49]. Given the fact that in the absence of any dimerization a gap can be opened only dueto frustration for α ≥ αc ≈ 0.24, one can see that in the (δ, α) parameter space the spin gap and themagnetic excitation spectrum in general can be quite complicated. Results of calculations for concretesets of parameters are shown for instance in Fig. 17. This figure will be discussed later in connection withthe possible observation of Raman active magnetic collective modes in the low temperature phase. As forthe short wavelength excitations, we mention that in general, for quite a wide range of parameters δ andα, the energies of the elementary triplet excitations at the zone boundary are not strongly renormalizedfrom πJ1/2, which is the value corresponding to the uniform NN AF spin chain.
The low temperature phase has been quantitatively explored by various techniques. INS data showthat below Tc there are two close-by gapped magnon excitations which have a large dispersion along theb-axis (inferred to be of about 80 meV - 645 cm−1) and the corresponding k = 0 values between 8 and11 meV (see the caption of Fig. 14 for a discussion) . The magnitude of the a-axis modulation is muchsmaller, of the order of only 1 meV, confirming weak inter-ladder interaction. We note that one of thespin gaps found by INS is situated at 8.3 meV (66.9 cm−1), an energy which, within error bars, is equalto the one corresponding to the very strong Raman active mode seen at 65.9 cm−1 in Fig. 11 below Tc.Note that the double folding of the branch corresponding to the 8.3 meV spin gap (shown in Fig. 14b)leads to the appearance of another Brillouin zone center feature with an energy of 10.9 meV (87.9 cm−1).The presence of spin-orbit coupling allows the observation of some of these elementary triplet excitationsalso in far IR  and ESR spectra . A low temperature gap of 8.13 meV (65.5 cm−1) is determinedwith high resolution by these two techniques.
Electronic Properties of α′-NaV2O5 19
Fig. 14. Inelastic neutron scattering data from Ref.  (a) Left panel: Constant energy scans along the chaindirection. The wavevector Qb is defined in units of 1/b. Right panel: Energy dispersion of the elementary tripletexcitation along the chain direction (b-axis); qb = Qb − 0.5. The empty and filled circles at qb = 0 in this figurecorrespond to data taken on two thermal neutron spectrometers, IN8 and IN22. (b) Dispersion along the a-axisfor Qb = 1 of the elementary triplet branch showing the folding of this excitation due to the unit cell doubling inthe direction perpendicular to the ladders. Consequently, its periodicity is π/a. The red line corresponds to theunfolded branch; note that its periodicity is 2π/a. According to the interpretation in Ref. , in the Brillouin zoneof the high temperature phase there is a second branch analogous to the one shown by the red line and very closein energy, whose dispersion is phase shifted by π/2. The reason this branch appears is because the superexchangeJ1 are slightly different in adjacent ladders as a result of charge/spin ordering. In the low temperature phase thissecond branch gets folded too (see Fig. 4 in Ref. ), and the data in (a) refers to this particular excitation. Inthe end, there are four Brillouin zone center modes corresponding to 8.3 (66.9) and 10.9 (87.9) meV (cm−1), fromthe first branch shown in panel (b) and to 9.1 (73.4) and 10.1 (81.5) eV (cm−1) from the second branch.
We observed so far that the transition at 34 K involves several aspects: (1) crystallographic distortionsleading to doubling of the in-plane lattice constants along and across the ladder legs as well as a quadru-pling of the unit cell in a direction parallel to the c-axis; (2) in-plane zig-zag charge ordering which has avery complicated pattern in a direction perpendicular to the plane; (3) development of gapped magneticbranches (with spin gaps in the 9 meV energy range) which are much more dispersive along the ladderlegs than in the transverse direction. The question is what is the driving force of this transition? Is it aspin-Peierls transition as it was initially thought, is it driven only by Coulomb forces which stabilize thezig-zag ordering, leading also to lattice distortions via electron-phonon coupling or does it occur mainlyas a result of a structural instability? Note that in the latter two scenarios the opening of a spin gapin the magnetic excitation spectrum is a by-product of the lattice/charge ordering rather than the maincause of the transition.
The arguments against an ordinary spin-Peierls scenario were mentioned in the introduction andthey rely mainly on the absence of magnetic field effects on Tc, the absence of other incommensuratestates at high fields and the observation of a large entropy release at the transition which could notbe accounted by the spin degrees of freedom alone. Seo and Fukuyama proposed in Ref.  a modelHamiltonian containing single dxy V orbitals and taking into account on-rung, ladder leg and inter-ladderhopping parameters t⊥, t‖ and txy (see Fig. 3), as well as on site (U) and nearest neighbor Coulombinteractions V⊥, V‖ and Vxy (these latter notations are in correspondence with the notations used for thehopping parameters). Three stable AF solutions were found within the Hartree approximation and theycorrespond to: (1) the uniform phase (all V atoms are equivalent, i.e. what is thought to be realized inthe high temperature phase); (2) the chain type having V4+ atoms on a given ladder leg and V5+ ions onthe other (which would correspond to the initial room temperature crystal structure determination );(3) the zig-zag type, which is the one shown in Fig. 12. It was found that for a large (and relevant) rangeof parameters, including the ones proposed in Ref. , the lowest energy state (above a small criticalvalue of the intersite Coulomb interaction defined as V = V⊥ = V‖ = Vxy/
√2) is one having zig-zag
order with alternate charge disproportionation on each rung. Depending on the relative magnitude of
20 A. Gozar and G. Blumberg
the hopping parameters it was proposed that the drop in susceptibility below Tc is related to a singletstate formation of essentially localized pairs of spins. The zig-zag order was also found consistent withthe observed in-plane unit cell doubling. As a result, the authors suggested that the charge ordering dueto Coulomb interaction is the driving force of the transition at 34 K in NaV2O5 .
Using a similar Hamiltonian except for excluding double occupancy of V dxy orbitals, equivalentto making U → ∞, a subsequent study confirmed the stabilization of the zig-zag pattern . Theauthors of Ref.  also pointed out that this kind of charge ordering along with inter-ladder correlationswill automatically lead to an alternation of the exchange integrals along the ladder direction, Ji,i+1 =J1(1+(−1)iδ), where i is a rung index. This alternation will open up a spin gap and lead to an exponentialdrop of the susceptibility below Tc. Another important point was related to the interaction betweencharges via lattice distortions: the zig-zag structure is also favored by the displacements of the rung Oatoms which are pushed by the large V 4+ ions.
More recent exact diagonalization results, see Ref. , also support the prominent role of the Coulombinteractions for the 34 K transition in NaV2O5 . The authors highlight the importance of phonons in thestabilization of the zig-zag structure, especially of the alternate c-axis displacements of the V atoms inthe low temperature phase, which were seen in X-ray data . It was found that the coupling of theelectrons to the lattice can substantially reduce the critical value of the intersite Coulomb repulsion (seethe previous paragraph) at which the formation of the charge ordered state occurs.
Interestingly, besides the low energy spin excitations arising as a result of dimerization, the charac-teristic low energy charge excitations are proposed to be soliton-like modes, similar to some degree to thespinons which are domain walls between degenerate ground state configurations, see Fig. 9. In this case,for an individual ladder there are two equivalent zig-zag patterns forming the ground state, the differencebetween them being a lattice translation with a high temperature lattice constant b. A low energy kink-like excitation will involve local on-rung electron hopping and will smoothly interpolate between the twodegenerate configurations, see for instance Fig. 6 in Ref. . One can conclude this section dedicatedto the nature of the low temperature phase by saying that both experimental and theoretical works arestrongly in favor of a transition driven by Coulomb interactions, with the spin gap formation playing onlya secondary role.
3.2 Observation of a folded triplet excitation. Selection rules and interpretation
Polarization properties and selection rules in magnetic fields – We discussed in the previoussection that INS data reported the existence of Brillouin zone center spin flip excitations around 11 meV.At low temperatures and in (ab) polarization we observe a relatively weak feature around 86 cm−1, seeFig. 15. What relatively weak means compared to other features seen in cross and parallel polarizationscan be inferred from in Fig. 18 where this feature is denoted by T in the lower left panel. In finiteexternal fields this feature has the following properties: it shows no shift for B parallel to the a-axis butwe observe a splitting for the other two orthogonal directions of the external magnetic field. Both theupward and downward dispersing branches change their energies in an approximately linear fashion, witha proportionality factor given by one Bohr magneton µB. This shows that we are looking at a S = 1excitation and we identify it with the elementary zone center triplet seen by neutron scattering. Note thatin finite fields there is an extra mode around 90 cm−1. This is a fully symmetric phononic feature whichappears because in finite magnetic fields, the orthorhombic (or even smaller) crystal symmetry leads to aFarady rotation of the polarization inside the sample preventing the observation of clean selection rules.In fact the finite field spectra were taken after the polarization optics were rotated in order to minimizethe intensity of strong features seen in parallel polarization (for instance the 66 cm−1 mode from Figs. 11and 18).
Fig. 15 reveals an interesting behavior of the 86 cm−1 mode. Because of the spin selection rules, Ramanscattering usually couples to singlet (S = 0) excitations. The observed magnetic field dependencies clearlyindicate the triplet nature of this mode. This is possible in the presence of spin-orbit coupling which mixesthe spin and orbital degrees of freedom, see the Introduction for a more detailed discussion. In what followswe try to identify the coupling mechanism responsible for the experimental observations from Fig. 15 aswell as the corresponding selection rules.
Electronic Properties of α′-NaV2O5 21
80 85 90
75 80 85 90 95
Raman shift (cm-1)75 80 85 90 95
0 2 4 6 8
B||a B||b B||c dispersions
Fig. 15. From left to right, the first three panels show Raman response at 5 K as a function of magnetic field. Eachspectrum is off-set by an amount equal to the value of the field at which is was taken. The colored symbols are dataand the thick dark grey lines through the data points are results of Lorentzian fits to the triplet component(s).The feature appearing around 90 cm−1 in finite fields is a phonon which exists also in the high temperature phase.Note that the 86 cm−1 mode splits for magnetic fields B ‖ b and B ‖ c but it does not shift for B ‖ a-axis. Panel(d) shows the dispersion with field of the 86 cm−1 mode for the three field configurations (squares for B ‖ a;triangles for B ‖ b and circles for B ‖ c).
The role of the antisymmetric Dzyaloshinskii-Moriya interaction – It is often possible tocapture the effects of certain spin-orbit interactions by writing effective spin Hamiltonians. Such a Hamil-tonian was inferred from macroscopic considerations in 1958 by Dzyaloshinskii  and two years later byMoriya , who derived a similar expression from a microscopic approach which needed superexchange(wavefunction overlap) and spin-orbit coupling as the only ingredients. If one writes down the most general
bilinear interaction between two spins at lattice sites i and j in the form∑
α,β Sαi Jαβ
ij Sβi and considers
only the antisymmetric part of the Jαβij tensor, one obtains the general form of the Dzyaloshinskii-Moriya
Dij · (Si × Sj) (4)
This type of interaction appears usually in crystals with lower symmetry and it is often responsible for thephenomenon of weak ferromagnetism. An example in this sense is the La2−xSrxCuO4 system discussedin more detail in .
The importance of the DM interaction was already suggested by ESR experiments which detecteda considerable anisotropy of the absorption lines with respect to the magnetic field orientation [52, 26].The direct observation of singlet-triplet transitions at low temperatures in ESR  and low frequencyIR absorption spectra  also proposed that the DM interaction is the mechanism which allows thecoupling of the photon field to single magnon excitations. We note that below Tc = 34 K, the localcrystal symmetry is low enough to allow the presence of DM type terms between neighboring spins.In a theoretical study, Valenti et al. studied Raman scattering in quasi-1D AF spin chains. The mainconclusion of this paper is that a single magnon excitation probed by Raman scattering has a very clearexperimental signature: it should show no splitting in an external magnetic field parallel to D and itshould split in two branches for a field perpendicular to the DM vector.
The authors of Ref.  also noted that there is no experimental confirmation of their predictionand so it is up to now to the best of our knowledge. Inspection of Fig. 15 shows that what we observeexperimentally resembles closely the theoretical predictions if D ‖ a. Although the Raman selection rules
22 A. Gozar and G. Blumberg
.) B || dJ
0 3 6 9B (Tesla)
B ⊥ d(b)
B || d(c)
0 3 6 9B (Tesla)
B ⊥ d(d)
Fig. 16. Energy levels and light couplings as a function of magnetic field for a system of two spins withDzyaloshinskii-Moriya interaction. The Hamiltonian reads JS1 · S2 + D · (S1 × S2) + gµBB · (S1 + S2) withD chosen parallel to the z axis. The way the energy levels split for B ‖ D, panel (a), and for B ⊥ D, panel (b),are illustrated for J = 20 and D = 12. Panels (c) and (d) show the moduli square of the nonvanishing matrixelements of the S1 · S2 operator between the ground state and the three excited states (the same color coding isused as on the left side of the figure).
for accessing the elementary triplet states may look complicated and were derived in Ref.  based on anon-trivial cluster-model approach, we believe that some understanding can be gained if we look at theproblem from the weakly coupled dimer limit. That is, let us assume that the ladders are magneticallydecoupled and in each individual ladder the alternation parameter δ from Eq. 3 is very close to unity.In this limit one deals in the zero order approximation with independent antiferromagnetically coupledspin dimers. Let us include an intra-dimer DM interaction of the form given by Eq. 4 and diagonalizethis two spin problem in the presence of an external magnetic field. The results, exemplified for J = 20and D = 0.6J (which are values not extracted from any experimental data), are shown in Fig. 16. Thissimple exercise is also useful for the understanding of some of the results in the SrCu2(BO3)2 chapter, where a slightly more complicated system (four spins instead of two) is used in order to understandthe low energy magnetism in the quantum spin system the SrCu2(BO3)2 orthoborate. However, in spiteof the additional complication, many of the features discussed here are more visible and apply to theorthoborate case.
Panels (a) and (b) show the energy levels as a function of magnetic field for two directions: perpen-dicular and parallel to the DM vector. In the absence of field and for D ≡ 0 we have a singlet at energy−3J/4 and a triple degenerate S = 1 excitation at J/4. A DM interaction (chosen parallel to the z-axis)in zero field will mix the singlet and the triplet states, in particular the vectors corresponding to zerocomponent of the z projection of the total spin operator Sz = Sz
1 + Sz2 . As a result the states with
Sz = ±1 will remain at J and the 1/√
2(| ↑>1 | ↓>2 ∓| ↓>1 | ↑>2) states (corresponding to the singletground state and excited |S = 1, Sz = 0 >≡ |1, 0 > state respectively) will repel each other. The |0, 0 >
ground state will have an energy −3J4 + J
1 + D2
≈ −3J4 − D2
4J for D J while the |1, 0 > state
will be at J4 + J
1 + D2
≈ J4 + D2
4J for D J . If the field is parallel to the DM vector, the
Sz = ±1 states will split with one Bohr magneton per Tesla while the other two states will not change
Electronic Properties of α′-NaV2O5 23
their energies. If the field is perpendicular to the DM vector the mixing of the states will be differentand this will lead to a different splitting of the triplet multiplet, see Fig. 16b. Although at high fields thedispersion with field is again linear, the derivative of the energy with respect to the field as B → 0 isvanishing in this second case. The curvature of the dispersion at small fields is a measure of the strengthof D.
Having in mind that the Fleury-Loudon coupling contains sums of scalar products of spins, see Eq. 2,in Fig. 16c-d we evaluated the moduli square of the matrix elements of the S1 · S2 operator and in thesetwo panels we show all the non-vanishing terms for both field configurations. In zero field the couplingis finite only for the |1, 0 > state. If B ‖ z no additional coupling appears and the intensity of the |0, 0 >↔ |1, 0 > transition is field independent. If B ⊥ z there will be a finite coupling to the up and downdispersing branches. The crossing points of intensities in panel (d) is also a measure of D. Overall, whatthese two panels say is that if the magnetic field is parallel to the DM vector one should see only onemode which does not change its energy with field, while if it is perpendicular to it two modes should beseen in finite fields, and both of them should shift with increasing field. The conclusions of this simplemodel are essentially the same as those of Ref.  which says that a local picture in terms of independentdimers is qualitatively appropriate.
According to the experimental results from Fig. 15a-d and the theoretical predictions from Ref. our data can be understood as a result of the Raman coupling to one magnon excitations through theDM interaction with D ‖ a-axis in the low temperature phase. A quantitative analysis of the intensitydependence is not possible because of the induced changes in the polarization directions inside the samplewhen magnetic fields are applied (changes that could not be controlled rigorously) as well as because of theappearance of the 90 cm−1 feature which obscured the upward dispersing branch. From the observed linear(within our resolution) magnetic field dependence of the modes energies as well as from the similar spectral
weights of the split triplet components at all measured fields in the B ‖ b and/or B ‖ c configurations (2 ≤B ≤ 8.9) we infer that possible non-linearities in the energy dispersions or strong variations in intensitiestake place below the value B = 2 T. Clearly, the intensity variations predicted in Fig. 16d are not seenin the experimental data which shows that the two peaks in panels (b) and (c) have similar intensities.We think that this discrepancy occurs because the actual spin structure is much more complicated thana simple ensemble of uncoupled spin dimers and higher order spin interactions and possibly inter-ladderinteractions have to be taken into account.
We clarified the existence of a single magnon excitation at 86 cm−1 in Raman scattering spectra.The feature is weak compared to other observed excitations in the Raman data. The question we wantto address in the following is whether we observe other magnetic modes, in the singlet channel, besidesphononic excitations. This is the topic of the following section.
3.3 Do we observe magnetic bound states below the two-particle continuum?
Excitations out of 1D S = 1/2 AF chains with dimerization and frustration – We arguedabove that the relevant spin Hamiltonian for an individual ladder is given by Eq. 3 so a closer look at themagnetic excitation spectrum of a dimerized and frustrated spin chain is useful. We discussed there thatany finite dimerization parameter δ and/or values of the frustration parameter α above a critical valuewill open up a spin gap ∆ = ∆(δ, α). Qualitatively, the dispersion of the elementary triplet (one magnon)excitation given by ε(k) looks like in Fig. 13b. The two triplet continuum (defined as the range of energiesω(k) = ε(k1) + ε(k1) with the wavevectors satisfying k = k1 + k2) will have a minimum at k = 0 andstarts from an energy ε = 2∆. It turns out that the Hamiltonian of Eq. 3 also allows for the existence oftwo triplet bound states, which means that at certain wavevectors there are two triplet excitations withenergies below the continuum [48, 49, 50].
An example of a perturbational calculation  of single and two triplet dispersions for certain pointsin the (δ, α) parameter space is shown in Fig. 17. Note that in these figures the wavevectors are on thevertical scales and the energies are on the horizontal axes. Panel (a) shows elementary triplet excitationsfor several points in the (δ, α) parameter space. The dispersion is similar to Fig. 13b, there is a rapidvariation of the zone center values but not much happens at the Brillouin zone center where the energiesare not far from πJ1/2 (note that the unit of energy in this figure is not J1 but J1(1 + δ)). Results for
24 A. Gozar and G. Blumberg
2 ππ ππ/b
)(a) (b) (c) (d)
Fig. 17. Results of perturbative calculations using continuous unitary transformations for the excitations of a 1DAF chain with dimerization and frustration (from Ref. ). The results shown here are for the NNN exchangeJ2 = αJ1 with α = 0.25(1−δ) and the energies are given in units of J1(1+δ). The parameter λ is defined in termsof the dimerization δ as λ = (1−δ)/(1+δ). (a) Elementary triplet dispersion ω(k) for λ = 0.3, 0.4, 0.5, 0.6 whichtranslates into (δ, α) = (0.54, 0.115); (0.43, 0.143); (0.33, 0.167); (0.25, 0.187). Panels (b) and (c) show two-tripletbound states (black lines) with total spin S = 1 and S = 0 respectively calculated for λ = 0.6 (δ = 0.25). Thelower bound of the two particle continuum is shown by the light blue line. (d) The ratio of the singlet (S = 0)bound states (at k = 0) to the value of the spin gap as a function of α (denoted by the authors of Ref.  by α0)for several dimerization parameters. The vertical line corresponds to the critical frustration where a gap opensin the spin excitation spectrum in the absence of any dimerization (see the discussion related to Fig. 9) and thehorizontal line denotes
the two-particle sectors are shown in panels (b) and (c) and one can see the continuum marked by thelight blue color. One important thing to note in these two figures is the occurrence of two-triplet boundstates whose dispersions are shown by black (solid, dashed or dash-dotted lines) lines. Panel (b) showsthe results for states in which two triplets are bound into a S = 1 state while panel (c) shows the samething but for triplets bound in a state having a total spin S = 0. For each case there are more than onebound states, the difference for the numerical parameters shown being that the binding energies of thetriplet bound states are finite only at finite values of k while for the singlet channel there is a branch splitfrom the continuum in the whole Brillouin zone.
Fig. 17d shows the ratio of the energy of lowest singlet bound state at the Brillouin zone center mS=0,with respect to the value of the elementary triplet gap ∆. The vertical line corresponds to the critical valueof α at which a frustration induced gap opens up in the absence of any dimerization δ. At αc, the aboveratio is mS=0/∆ =
√3 (the horizontal line refers to this value) and its value decreases with increasing
frustration. Note that at α = 0, mS=0/∆ ≈ 2, and this is true irrespective of the chosen values for δwhich means that it is the frustration which leads to finite binding energies of the singlet bound states.One interesting point which is not shown in panel (d): there exists a singular point, the Majumdar-Ghoshpoint given by (δ, α) ≡ (0, 0.5) (see the discussion of Fig. 9), where mS=0/∆ equals unity. At this pointthe single magnon and the two-magnon bound state are degenerate, which is a remarkable property ofthe Hamiltonian of Eq. 3 .
Experimental observations and discussion – How is this discussion related to our experimentalfindings in NaV2O5 ? In Fig. 18 we show several Raman spectra with the purpose of emphasizing thenew excitations which appear below the phase transition. We discuss first an aspect related to the crystalsymmetry in the low temperature phase and illustrated in panels (c) and (d) of this figure. We show therefour Raman spectra, two in (aa) polarization at 300 and 4 K, Fig. 18c, and two in (ab) polarization at thesame two temperatures, Fig. 18d. In the high temperature phase the V-Orung stretching mode [23, 25]is present at 969 cm−1 in parallel polarizations, but not in (ab) geometry and, therefore it is a fullysymmetric excitation of the Pmmn space group. Below Tc this mode acquires a second component, seenat 948 cm−1, due to the in-plane unit cell doubling, i.e. we assign it to a folded phononic branch. More
Electronic Properties of α′-NaV2O5 25
(aa) 4 K
0 50 100 150 200
(ab) 4 K
Raman shift (cm-1)
940 960 980
Fig. 18. Low energy Raman scattering spectra in (aa) (upper panels) and (ab) (lower panels) polarizations at4, 40 and 300 K measured using the ωin = 1.92 eV excitation. Below about 34 K many new resonances appearin the 0-200 cm−1 region. The arrows at the top correspond to the energies of the elementary triplet excitationdetermined by high resolution IR  and ESR  studies and twice that value. The 968 cm−1 phonon in paralleland cross polarization is shown on the right. Panel (d) shows that below Tc a folded counterpart appears whichis seen in both (aa) and (ab) polarizations indicating a lower crystal symmetry.
importantly, both the 968 and 949 cm−1 excitations are seen not only in (aa) but also in (ab) polarization.The simultaneous presence of these modes in both the diagonal and off-diagonal components of the Ramantensor indicates that in the low temperature phase the double reflection symmetry of the Fmm2 group isbroken. Our data confirm the resonant X-ray data  which argues for a lower (monoclinic) symmetrybelow Tc.
We comment now on the spectra shown in Fig. 18a-b. In panel (a) we show the emergence of new(aa) polarized collective modes in the low temperature phase and several of them are indexed by letters:A (56.9cm−1), B (105.0 cm−1), C (131.2 cm−1), D (164.0 cm−1) and E (200.4 cm−1). In panel (b) wesimilarly marked the modes T (86.5cm−1) and F (149.0cm−1) seen in the (ab) polarized spectra. Thislist of modes does not exhaust all of the new excitations appearing in the low temperature phase buthighlights a few of them which are of importance for the following discussion. What is the origin ofthese new modes? Are they phonons, are they magnetic or are they some collective topological chargeexcitations of the type described in Ref. . While not excluding the latter option, it seems that theobservation of purely charge modes is less probable because it involves higher energies of the order intersiteCoulomb interactions which are of the order of eV’s [19, 54]. Moreover, the characteristic energy scales
26 A. Gozar and G. Blumberg
60 64 68
Raman Shift (cm-1)
100 104 108
1.6 2 2.4
Photon energy (ωin)
1.6 2 2.4
) / I
(a) (b) (c)
Fig. 19. Panels (a) and (b) display the T = 5 K Raman spectra showing the magnetic field (in)dependence ofthe 66 and 105 cm−1 resonances which appear below the transition. In both cases a shift of about 0.9-1 cm−1 wasobserved as the magnetic field was varied from 0 to 8.9 T. (c) Integrated intensity of the 66 (empty squares) and105 cm−1 (filled triangles) modes at 5 K as a function of the incoming photon energies ωin. The inset of this panelshows that the ratio of the integrated intensities of these two modes depend only slightly on ωin (as opposed tothe data shown in Fig. 6, the data in the main panel were not corrected for the optical properties of the material;however these effects cancel out in the ratio because these modes are very close in energy).
of these excitations (0-25 meV) can be better related either to magnetic excitations seen in ESR, farIR or INS experiments (see Fig. 14) or (in the context of existing lattice instabilities which drive the34 K transition) to the folding of low energy zone boundary phonons in the high temperature phase.Accordingly, we will focus here on the possibility of observing phonons or single/multi-triplet magneticexcitations [48, 59].
We discuss here the spin excitations scenario. This picture draws its appeal primarily from the factthat the Hamiltonian of Eq. 3, which seems to be a good description for the staggered spin configurationin the low temperature phase, allows for a multitude of magnetic bound states, both in the singlet andtriplet channels, see Fig. 17. First, we note that some of the new resonances observed below the transitionare definitely magnetic. In Fig. 15 we showed that the 86.5 cm−1 excitation, denoted by T in Fig. 18,is a S = 1 magnon. The singularity seen at 131.2 cm−1 (16.27 meV) in Fig. 18a-b situated at twicethe energy of the spin gap value of 65.5 cm−1 (8.13 meV) and the continuum present from above thisfrequency as opposed to the clean gap seen for ω ≤ 130 cm−1 (except for a few resonances) leaves littledoubt that the mode C marks the onset of the two-triplet continuum of excitations. How about themost prominent excitations denoted by A and B in Fig. 18a? The similar resonance profile of these twoexcitations shown in Fig. 19 indicates that they have a common origin. It is interesting to remark thatthe energy of mode A coincides with the energy of the spin gap determined with high resolution in ESRand IR absorption data [51, 52]. Can this excitation be the k = 0 elementary triplet? Panels (a) and(b) in Fig. 19 show that neither mode A nor mode B splits or shifts by more than 1 cm−1 in appliedmagnetic fields up to 8.9 T (and we checked that this is true for any direction of the applied magneticfield). Moreover, if these excitations were S = 1 triplets and the same spin-orbit interaction would insurethe coupling to them as for mode T, one could not explain that the spectral weight of mode A is morethan two orders of magnitude higher than that of mode T.
The arguments above seem to exclude the possibility that modes A and B are triplet excitationsbut the possibility that they are bound states in the singlet sector still needs to be explored. The ratioωB/∆ = 1.59 appears to qualify mode B for a singlet bound state according to Fig. 17d. How about modeA, can it be also a singlet bound state? As discussed previously, a singlet bound state degenerate withthe spin gap is only realized for a singular combination of parameters, (δ, α) ≡ (0, 0.5). It deserves furtherargumentation why this set of values is realized in the low temperature phase of NaV2O5 . However,assuming that this is the case, one could assign mode B to the folded counterpart of mode A. In this
Electronic Properties of α′-NaV2O5 27
scenario one could also argue that the magnetic frustration may be the driving force of the transitionat 34 K in the following way . The tendency for zig-zag ordering increases the value of the NNNfrustrating interaction J2. At 34 K, α = J2/J1 reaches the critical value αc (see the caption of Fig. 17)and a gap opens in the magnetic excitation spectrum. Further cooling will push α close to 0.5 and thesinglet bound state gets very close (practically degenerate) to the spin gap. Going into more details ofthis pictures some of the other excitations can be understood as combination modes or continuum edges.For instance, based on energy considerations, one can say that F = A + B, H = B + B or that mode Fin Fig. 18b is the A + T continuum edge.
However, the fact that the physics of the Majumdar-Ghosh point is realized for a singular combinationof parameters makes this appealing scenario less probable. The variety of selections rules which have beenexperimentally observed in Raman, ESR and IR data still needs to be explained. The second possibilityis to assign the main new features appearing below Tc in the 0-200 cm−1 energy range to folded phonons.In fact, this scenario is supported by the small but finite shift observed in Fig. 19a-b. This is what oneexpects in a simple two level system: one phonon, one close by magnon along with some off-diagonal matrixelements because of a non-vanishing spin-phonon interaction. As expected, the shift of the 65.9 cm−1 mode(of about 0.8 cm−1) is slightly higher than the shift of the 105 cm−1 mode (of abut 0.5 cm−1) which isfurther apart in energy from the spin gap value. Based on lattice dynamical calculations and the relativetemperature dependence of the spin gap seen in ESR data  and that of the energies of measured IRactive modes, a more recent study also argues for the phononic nature of modes A and B .
We conclude this section by saying that many features of the transition at 34 K in NaV2O5 are stillunder debate and more than just a clarification is needed regarding the nature of the observed excitationsor the effects of the electron-phonon interactions.
In this chapter we studied electronic excitations in NaV2O5 by Raman scattering and the transition takingplace at Tc = 34 K. From the description of the crystal structure and the discussion of the electronicproperties as seen by various techniques we showed that NaV2O5 can be thought of as an array of quasione-dimensional (1D) two-leg ladders at quarter filling factor. Two models were proposed to capture theessential physics of the magnetic degrees of freedom: one for the high temperature phase (Heisenbergchains with nearest and next nearest antiferromagnetic interactions, see Eq. 1), and another model forthe low temperature phase (Heisenberg chains with dimerization and frustration, see Eq. 3).
Three main topics were discussed. The first was related to a broad continuum of excitations found inthe 200-1500 cm−1 range and peaked around 680 cm−1 in parallel polarizations. In literature a magneticorigin of this feature was ruled out and a scenario involving crystal field excitations was proposed instead.The resonant Raman profile of this excitation, the polarization selection rules and the presence of itsovertone in resonance conditions allowed us to conclude that the origin of this feature is magnetic. Moreprecisely, we proposed that it arises as a result of light coupling to multi-spinon Raman excitations.Within this scenario we also argued for a scenario explaining the puzzling temperature dependence ofthe magnetic continuum in terms of an increasing role of next nearest neighbor frustration and in thecontext of a strongly fluctuating low temperature phase.
The second topic was related to the observation of a folded S = 1 magnetic mode which displayedvery clear selection rules as a function of the magnetic field orientation, see Fig. 15. We proposed thatthe coupling of the photon field to this excitation takes place via the antisymmetric, Dzyaloshinskii-Moriya (DM), interaction which, in a simple dimer model, can also explain the observed selection rules:no splitting or shifts for magnetic fields parallel to the DM vector and the observation of two (upwardand downward) dispersing branches for fields perpendicular to the DM vector.
Finally, we discussed the nature of several new resonances seen below Tc and focussed on the possibil-ities that they are either folded phonons or singlet bound states of two triplet excitations. In particularwe emphasized the existence of two modes at 66 and 105 cm−1, the first one being degenerate with oneof the spin gap modes. In the spin excitations scenario we proposed a model in which frustration hasa determinant role. However, in order to accommodate theoretical results with the observed energies, a
28 A. Gozar and G. Blumberg
very particular set of parameters characterizing the dimerized and frustrated spin chains (the Majumdar-Ghosh point) had to be invoked. The above argument and the small energy shifts in magnetic fields up to9 T suggested that the strong mode degenerate with the elementary triplet as well as the 105 cm−1 modeare phonons. The conclusion of our study is that many features of the spin/charge and lattice dynamicsin NaV2O5 are still to be understood.
Acknowledgments – We acknowledge discussions and collaborations with B. S. Dennis, M. V. Klein,U. Nagel, T. Room, A.M. Sengupta and S. Trebst. The crystals were provided by P. Canfield.
[∗] E-mail: [email protected]. M. Isobe and Y. Ueda, J. Phys. Soc. Jpn. 65, 1178 (1996).2. A. Gozar and G. Blumberg, ”Collective Spin and Charge Excitations in (Sr,La)14−xCaxCu24O41 Quantum
Spin Ladders”, also in the present volume.3. E. Pytte, Phys. Rev. B 10, 4637 (1974); M. C. Cross and D. S. Fisher, Phys. Rev. B 19, 402 (1979).4. L. N. Bulaevskii, A. I. Buzdin and D. I. Khomskii, Solid State Commun. 27, 5 (1978); M. C. Cross, Phys.
Rev. B 20, 4606 (1979).5. M. Hase, I. Terasaki and K. Uchinokura, Phys. Rev. Lett. 70, 3651 (1993).6. For a review of CuGeO3 properties see J. P. Boucher and L. P. Regnault, J. de Physique I 6, 1939 (1996).7. Y. Fujii et al., J. Phys. Soc. Jpn. 66, 326 (1997).8. W. Schnelle, Yu. grin and R. K. Kremer, Phys. Rev. B 59, 73 (1999).9. A. Damascelli, Ph. D. Thesis, 1999.
10. J. Hemberger et al., Europhys. Lett. 42, 661 (1998).11. P. A. Carpy and J. Galy, Acta Cryst. B 31, 1481 (1975).12. S. Grenier et al., Phys. Rev. B 65, R180101 (2002); Y. Joly, S. Grenier and J. E. Lorenzo, Phys. Rev. B 68,
104412 (2003).13. M. J. Konstantinovic et al., Phys. Rev. B 65, 012404 (2002).14. H. Smolinski et al., Phys. Rev. Lett. 80, 5164 (1998).15. A. Meetsma et al., Acta Cryst. C 54, 1558 (1998).16. J. Ludecke et al., Phys. Rev. Lett. 82, 3633 (1999).17. T. Ohama et al., Phys. Rev. B 59, 3299 (1999); T. Ohama et al., J. Phys. Soc. Jpn. 69, 2751 (2000).18. K. Kobayashi et al., Phys. Rev. Lett. 80, 3121 (1998).19. M. V. Mostovoy and D. I. Khomskii, Solid State Commun. 113, 159 (2000); M. V. Mostovoy, D. I. Khomskii
and J. Knoester, Phys. Rev. B 65, 064412 (2002).20. D. C. Johnston et al., Phys. Rev. B 61, 9558 (2000).21. C. Presura et al., Phys. Rev. B 61, 15762 (2000); C. Presura et al., Phys. Rev. B 62, 16522 (2000).22. A. Damascelli et al., Phys. Rev. Lett. 81, 918 (1998); A. Damascelli et al., Phys. Rev. B 61, 2535 (2000).23. S. A. Golubchik et al., J. Phys. Soc. Jpn. 66, 4042 (1997); Z. V. Popovic et al., Solid State Commun. 110,
381 (1999); M. N. Popova et al., J. Exp. Theor. Phys. 88, 1186 (1999).24. M. J. Konstantinovic et al., Phys. Stat. Sol. 215, 661 (1999).25. M. J. Konstantinovic et al., J. Phys.: Condens. Matter 11, 2103 (1999); M. J. Konstantinovic et al., Solid
State Commun. 112, 397 (1999).26. H. Nojiri et al., J. Phys. Soc. Jpn. 69, 2291 (2000).27. M. Fischer et al., Phys. Rev. B 60, 7284 (1999).28. M. J. Konstantinovic et al., Phys. Rev. B 65, 012404 (2001); M. J. Konstantinovic et al., Phys. Rev. B 65,
245103 (2001).29. M. N. Popova et al., Phys. Rev. B 65, 144303 (2002).30. P. A. Fleury and R. Loudon, Phys. Rev. 166, 514 (1968).31. B. S. Shastry and B. I. Shraiman, Phys. Rev. Lett. 65, 1068 (1990); B. S. Shastry and B. I. Shraiman, Int.
J. of Mod. Phys. B, 5, 365 (1991).32. B. Grenier et al., Phys. Rev. Lett. 86, 5966 (2001).33. P. H. M. van Loosdrecht et al., Phys. Rev. Lett. 76, 311 (1996).34. L.D. Faddeev and L.A. Takhtajan, Phys. Lett. A 85, 375 (1981); J. des Cloizeaux and J. J. Pearson, Phys.
Rev. 128, 2131 (1962).35. K. P. Schmidt and G. S. Uhrig, Phys. Rev. Lett. 90, 227204 (2003); C. Knetter et al., Phys. Rev. Lett. 87,
Electronic Properties of α′-NaV2O5 29
36. G. Castilla, S. Chakravarty and V. J. Emery, Phys. Rev. Lett. 75, 1823 (1995).37. C. K. Majumdar and D. K. Ghosh, J. Phys. C 3, 911 (1970); J. Math. Phys. (N.Y.) 10, 1388, (1969).38. A. Gozar and G. Blumberg, ”Collective Magnetic Excitations in SrCu2(BO3)2 ”, also in the present volume.39. R. R. P. Singh, P. Prelovsek and B. S. Shastry, Phys. Rev. Lett. 77, 4086 (1996).40. V. N. Muthukumar et al., Phys. Rev. B 54, R9635 (1996).41. W. Brenig, Phys. Rev. B 56, 2551 (1997).42. A. V. Chubukov and D. M. Frenkel, Phys. Rev. Lett. 74, 3057 (1995); Phys. Rev. B 52, 9760 (1995).43. G. Blumberg et al., Phys. Rev. B 53, R11930 (1996).44. R. R. P. Singh et al., Phys. Rev. Lett. 62, 2736 (1989).45. J. C. Bonner and M. E. Fisher, Phys. Rev. 135, A640 (1964).46. S. van Smaalen et al., Phys. Rev. B 65, R060101 (2002).47. K. Ohwada et al., Phys. Rev. Lett. 87, 086402 (2001).48. S. Trebst, Ph. D. Thesis, Bonn University, 2002.49. G. S. Uhrig and H. J. Schulz, Phys. Rev. B 54, R9624 (1996); G. Bouzerar, A. P. Kampf and G. I. Japaridze,
Phys. Rev. B 58, 3117 (1998); S. Trebst et al., Phys. Rev. Lett. 85, 4373 (2000); C. J. Hammer, W. Zhengand r. R. P. Singh, Phys. Rev. B 68, 214408 (2003).
50. K. P. Schmidt, C. Knetter and G. S. Uhrig, Phys. Rev. B 69, 104417 (2004).51. T. Room et al., Phys. Rev. B 69, 144410 (2004).52. S. Luther et al., J. Phys. Soc. Jpn. 67, 3715 (1998).53. H. Seo and H. Fukuyama, J. Phys. Soc. Jpn. 67, 2602 (1998).54. M. Aichhorn et al., Phys. Rev. B 69, 245108 (2004); E. Ya. Sherman et al., Phys. Rev. B 48, 648 (1999).55. I. Dzyaloshinskii, J. Phys. Chem. Solids 4, 241 (1958).56. T. Moriya, Phys. Rev. 120, 91 (1960).57. A. Gozar, B.S Dennis, G. Blumberg, S. Komiya, and Y. Ando, Phys. Rev. Lett. 93, 027001 (2004).58. R. Valenti, C. Gros and W. Brenig, Phys. Rev. B 62, 14164 (2000).59. G. Blumberg et al., unpublished.